Download presentation

Published byZechariah Dabney Modified over 3 years ago

1
**Peculiar magnetism of the FeAs – grand parent of the iron-based superconductors**

A. Błachowski1, K. Ruebenbauer1, J. Żukrowski2, and Z. Bukowski3 1 Mössbauer Spectroscopy Division, Institute of Physics, Pedagogical University, Cracow, Poland 2 Department of Solid State Physics, Faculty of Physics and Applied Computer Science, AGH University of Science and Technology, Cracow, Poland 3 Institute of Low Temperature and Structure Research, Polish Academy of Sciences, Wrocław, Poland This work was supported by the National Science Center of Poland, Grant DEC-2011/03/B/ST3/00446 XVI KKN - XVI National Conference on Superconductivity October 7-12, 2013: Zakopane, Poland Seminarium Instytutu Fizyki UP, Kraków, 25 października 2013 r. (piątek): sala 513: 9.35

2
**Mössbauer Spectroscopy Laboratory at MSD Institute of Physics, Pedagogical University Cracow, Poland**

4
**Mössbauer Spectroscopy**

-ray energy is modulated by the Doppler effect due to the source motion vs. absorber Mössbauer spectrum 1 mm/s 48 neV

5
**Hyperfine Interactions**

Isomer Shift Quadrupole Splitting Magnetic Splitting 57Fe Mössbauer spectra B = 10 T Electron Density Electric Field Gradient Magnetic Hyperfine Field

6
**Electric Field Gradient + Magnetic Hyperfine Field**

B = 10 T = 0° = 90°

7
**A bit of formalism Relevant hyperfine Hamiltonian:**

Choice of the “convenient” reference frame: Transition and parameter dependence of the Hamiltonians:

8
**For such axial ellipsoid aligned with the Cartesian **

Lattice dynamics and transition intensity corrections: Thermal ellipsoid for FeAs: For such axial ellipsoid aligned with the Cartesian quantization axes one has single anisotropy parameter. For the present case ellipsoid is flattened along y-axis.

9
**Spiral structure of the magnetic hyperfine field**

Parameterization of the spiral field:

10
**Iron-arsenic phase diagram**

Landolt-Börnstein New Series IV/5

11
**Structure of FeAs Orthorhombic structure The Pnma symmetry group**

Arrows show Pna21 distortion Quantization axes: abc - xyz All Fe atoms are equivalent within Pnma Thermal ellipsoid is flattened along b-axis [0 k+1/2 0] iron and [0 k 0] iron Orientation of magnetic spirals

12
**p-T phase diagram of FeAs**

J. R. Jeffries et al., Phys. Rev. B 83, (2011)

13
**Magnetic structure of FeAs**

Polarized neutron scattering results E. E. Rodriguez et al., Phys. Rev. B 83, (2011)

14
**Low temperature spectra of FeAs**

15
**Anisotropy of the hyperfine magnetic fields (spiral projections onto a-b plane) in FeAs**

Left column shows [0 k+1/2 0] iron, right column shows [0 k 0] iron. Ba and Bb - iron hyperfine field components along the a-axis and b-axis, respectively. Orientation of the EFG and hyperfine magnetic field in the main crystal axes Average hyperfine fields <B> for [0 k+1/2 0] and [0 k 0] irons. Tc - transition temperature - static critical exponent

16
**FeAs Spectral shift S and quadrupole coupling constant AQ**

versus temperature for [0 k+1/2 0] iron and [0 k 0] iron. Line at 72 K separate magnetically ordered region from paramagnetic region. Relative recoilless fraction <f>/<f0> versus temperature Green points correspond to magnetically ordered region. Red point is the normalization point. Inset shows relative spectral area RSA plotted versus temperature.

17
**Anisotropy of the recoilless fraction - FeAs**

Anisotropy disappears in the magnetic region

18
**Spectra in the external field anti-parallel to the beam - FeAs**

Model 1 (different electron densities) is preferred, as for Model 2 one obtains unphysical diamagnetic „susceptibility”. There is significant anisotropy of the „susceptibility” even high above transition temperature.

19
**High temperature spectra of FeAs**

Model 1 Saturation of the recoilless fraction anisotropy above RT is an indication of the onset of the quasi-harmonic behavior. Arsenic starts to evaporate at 1000 K and under vacuum leading to the Fe2As phase – irreversible process.

20
Conclusions The iron hyperfine field along the electronic spin spiral varies enormously in amplitude in the magnetically ordered region. The pattern resembles symmetry of 3d electrons in the a-b plane with the significant distortion caused by the arsenic bonding p electrons. Another unusual feature is strong coupling between magnetism and lattice dynamics i.e. very strong phonon-magnon interaction. Static critical exponents suggest some underlying transition leading to the magnetic order. Due to the lack of the structural changes one can envisage some subtle order-disorder transition with very small latent heat and hysteresis driven by the itinerant charge/spin ordering. The sample starts to loose arsenic at about 1000 K under vacuum, what might be explanation for the specific heat anomaly observed at high temperature.

Similar presentations

OK

Vortex Lattice Anisotropy in Magnesium Diboride Morten Ring Eskildsen Department of Physics University of Notre Dame.

Vortex Lattice Anisotropy in Magnesium Diboride Morten Ring Eskildsen Department of Physics University of Notre Dame.

© 2018 SlidePlayer.com Inc.

All rights reserved.

To ensure the functioning of the site, we use **cookies**. We share information about your activities on the site with our partners and Google partners: social networks and companies engaged in advertising and web analytics. For more information, see the Privacy Policy and Google Privacy & Terms.
Your consent to our cookies if you continue to use this website.

Ads by Google

Ppt on operating system architecture Ppt on wireless power transmission system Ppt on combination of resistance bands Ppt on solar system download Ppt on holographic technology videos Dilutive securities and earnings per share ppt online Ppt on lunar and solar eclipse Ppt on water pollution act Ppt on rockets and satellites Ppt on rational numbers for class 8 free download